Summarize this article in one sentence.
A degreasing solution is recommended for oily or heavily handled silver. If there is oxidization on the surface, you may need to place the silver in a pickle solution before soldering. Optionally, you may use 1000 grit sandpaper to make a rougher surface for joining. Prepare the flux according to instructions on the packaging, if it is not ready to use. Use a small paintbrush to apply this flux onto the silver object(s). Some people apply flux only where the solder will be present, in order to limit the amount of solder that flows to the wrong place. Others prefer to apply the flux over a larger area to minimize the risk of fire damage, but this is not recommended for beginners. Using a small amount of flux in a separate container is recommended, as repeatedly dipping a brush into the original bottle may add dirt and affect its function. Lay the two components next to each other on the soldering brick. Position them exactly as you want them to be joined, noting that they must be physically touching to be joined properly. Use a pair of tweezers to pick up a solder chip and gently place it on one end of the crack or gap to be joined. Once melted, the solder will be drawn by the heat anywhere flux was applied, so you do not need to cover the entire length of the gap. Light your torch and adjust the heat to its highest setting. Begin by holding the torch about 4 inches (10 cm) away from the joint, moving it constantly in small circles to ensure even heating of all components. Slowly move the flame closer to the joint, focusing on the metal objects near the solder, not the solder itself. When the solder reaches its melting point, it will quickly melt and be pulled onto the fluxed areas of the silver.  If one of the objects to be joined is thicker than the other, heat the thicker object from the back until the solder starts to melt, then heat the thin object briefly.  Use tweezers if necessary to hold the objects in place, but place them on the far end of the silver, away from the flame. You may need to hold down small, thin areas of the silver to provide a heat sink, preventing the thin area from melting. Let the object cool for a minute, then cool it further by dipping it into a water bath. The "pickle" solution described in the work area section is an acidic bath used to clean the jewelry after soldering. Lower the silver into this bath using copper tongs, and leave it for a few minutes to remove the flux and oxidization. Avoid all contact with your skin, clothing, or steel tools, as the pickle bath can be corrosive. Rinse the newly joined silver with water.  Pat dry with a clean cloth. If the process was completed correctly, the silver should remain joined permanently.

Summary:
Clean the silver. Apply flux to the joint. Position your silver components to be joined. Position the solder onto the joint. Heat the objects until the solder melts. Dip the object in water, then immerse it in a pickle solution. Rinse the silver.